BODIPY as building blocks for Near
InfraRed-Active Organic Compounds
Zur Erlangung des akademischen Grades Doktor der Naturwissenschaften
(Dr. rer. nat.)
eingereicht an der Fakultät für Mathematik und Naturwissenschaften der Bergischen Universität Wuppertal
Benedetta Maria Squeo
The PhD thesis can be quoted as follows: urn:nbn:de:hbz:468-20181204-140514-6
Prof. Dr. Ullrich Scherf and Dr. Christos L. Chochos.
This project has received funding from the European Community’s Seventh Framework Programme (FP7/2007-2013) under the Grant Agreements n° 607585 project OSNIRO.
1. Supervisor: Prof. Dr. Ullrich Scherf, Bergische Universität Wuppertal. 2. Reviewer: Dr. Christos L. Chochos,
- Advent Technologies SA
- Institute of Biology, Medicinal Chemistry & Biotechnology, National Hellenic Research Foundation
BODIPY (4,4-difluoro-4-bora-3a,4a-diaza-s-indacene) dyes are promising building blocks for the synthesis of NIR organic materials. Compared to other dye classes, these systems offer unique attractions such as excellent thermal/photochemical stability, intense absorption/emission profiles, negligible triplet-state formation, and small Stokes shifts. Their optoelectronic and semiconductor properties can be finely tuned via facile synthetic modifications on the dipyrromethene core.
In this PhD thesis new organic NIR materials (both π-conjugated polymers and small molecules) based on α,β-unsubstituted meso-positioning thienyl BODIPY have been developed, and their optoelectronic properties and their performances when applied in organic light emitting diodes and organic solar cells have been characterized and evaluated.
In more details, on the one hand donor-acceptor quarterthiophene-BODIPY polymers have been synthesized and the dependence of their optoelectronic, electrochemical and charge transporting properties of the resulting α,β-unsubstituted meso-positioning thienyl BODIPY quaterthiophene-based polymers from the alkyl side chain position have been studied. Tail-to-tail (TT) positioning of the alkyl side chains at the two central thiophenes of the quaterthiophene segment results in lower Eg
, higher energy levels and increased hole mobility as compared to head-to-head (HH) positioning. However, even though the synthesized polymers exhibit high electron affinity, higher even than that of the fullerene PC71BM, they present only p-type behavior in field effect transistors
(FETs) independent of the alkyl side chain positioning. Furthermore, one of the synthesized copolymers containing a vinylene bond in the middle of the quarterthiophene segment exhibits a panchromatic absorption spectrum ranging from 300 nm to 1100 nm and an optical band gap around 1 eV, suitable for near infrared (NIR) organic photovoltaic applications as electron donor. Preliminary power conversion efficiency (PCE) in bulk heterojunction (BHJ) solar cells of 1.1% in polymer:[6,6]-phenyl-C71-butyric acid methyl ester (PC71BM) [1:3 weight
ratio] has been achieved, demonstrating very interesting and promising photovoltaic characteristics, such as good fill factor (FF) and open circuit voltage (Voc).
On the other hand, BODIPY unit have been symmetrically conjugate with oligothienyls in a “metal-free” A-D-A (acceptor-donor-acceptor) oligomer emitting in the near-infrared (NIR) thanks to the delocalisation of the BODIPY low-lying lowest unoccupied molecular orbital (LUMO) over the oligothienyl moieties, as confirmed by density functional theory (DFT). A PL efficiency of 20% in the solid
(OLEDs) emitting at 720 nm. We achieved external quantum efficiencies (EQEs) up to 1.1%, the highest value recorded so far by a “metal-free” NIR-OLED not intentionally benefitting from triplet-triplet annihilation. These results demonstrate for the first time the promise of A-D-A type dyes for NIR OLEDs applications thereby paving the way for further optimization.
1. Introduction ………...…1
1.1. Near InfraRed materials ………...…. 1
1.1.1. Class of NIR materials………....…....1
1.1.2. Application of NIR materials………..…...2
1.2. Molecular design and energy gap engineering……….…….4
1.2.1. Intrinsic Energy Bandgap……….…….4
1.2.2. Effect of conjugation length and aggregation……….……..7
1.2.3. Donor-Acceptor approach……….…….…8
1.3. BODIPY dyes ……….……….….9
2. BODIPY Polymers ………..……13
2.1. Cross-coupling reactions for the synthesis of BODIPY-based polymers and small molecules ………...…13
2.2. Results and discussion………....15
2.2.1. Theoretical calculations………15
2.2.2. Synthesis of α,β-unsubstituted meso positioning BODIPY precursors……….18
2.2.3. Synthesis of polymers………20
18.104.22.168. Synthesis of TBDPTV……….20
22.214.171.124. Synthesis of BODIPY qTo, BODIPY qTi and CB06……...21
2.2.4. Electrochemical characterization………....23
2.2.5. Optical characterization………...26
2.2.6. Charge Transporting properties of BODIPY qTo and BODIPY qTi……….34
2.2.7. Photovoltaic properties of TBDPTV………...38
3. BODIPY Small Molecules ………...44
3.1. Introduction ………...44
3.2. Results and Discussion………...46
3.2.1. Synthesis of α,β-unsubstituted bromo-BODIPY………46
3.2.2. Synthesis od A-D-A small molecule NIRBDTE………..47
3.2.3. Electrochemical and Theoretical characterization………48
5. Experimental Data………...61 5.1. Instrument……….61 5.2. Synthesis……… 66 5.2.1. 2,2'-((5-octylthiophen-2-yl)methylene)bis(1H-pyrrole) (1)……...…68 5.2.2. 8-octylthiophene BODIPY (2)………....70 5.2.3. 2,6-dibromo-8-octylthiophene BODIPY (3)………..72 5.2.4. 5,5-difluoro-10-(5-octylthiophen-2-yl)-2,8-di(thiophen-2-yl)-5H-4λ4,5λ4 -dipyrrolo[1,2-c:2',1'-f][1,3,2]diazaborinine (4)………...74 5.2.5. 2,8-bis(5-bromothiophen-2-yl)- 5,5-difluoro-10-(5-octylthiophen-2-yl)-2,8-di(thiophen-2-yl)-5H-4λ4,5λ4-dipyrrolo[1,2-c:2',1' f][1,3,2]diazaborinine (5)………..78 5.2.6. 2,2'-((5-bromothiophen-2-yl)methylene)bis(1H-pyrrole)(6)……….80
5.2.7. Bromo functionalized-BODIPY monomer (7)………..81
5.2.8. Synthesis of NIRBDTE………..84 5.2.9. Polymer BODIPY-qTo………...85 5.2.10. Polymer BODIPY-qTi………..87 5.2.11. Polymer CB06………..89 6. Bibliography………..91 7. Curriculum Vitae……….96
Organic π-conjugated materials have attracted a tremendous academic and industrial interest in the last decades1–4. Thanks to their optoelectronic properties, nowadays these compounds are used as active material in several applications such as organic field effect transistors (OFETs)5–9, organic light emitting devices (OLEDs)a10–13, organic photovoltaics (OPVs)14–20, bio-imaging21,22, organic solid lasers23, and many others24.
1.1 Near Infrared materials
The infrared (IR) radiation is electromagnetic radiation with wavelength longer than those of visible light, but shorter than microwave. The bound between visible light and infrared radiation is not clearly defined. Generally we can consider the infrared radiation the one ranging between 700 nm and 10 μm, and more specifically near infrared (NIR) region the one between 700 nm and 2500 nm.
1.1.1. Classes of NIR materials
The characteristic features of the NIR materials are that they absorb, emit and generally interact with NIR light under external stimulation like electromagnetic field, photoexcitation and chemical reaction and they can be divided in two classes the inorganic and the organic materials.
Among the inorganic compounds, semiconductor nanocrystals (NCs) of II-IV, III-V and IV-VI group, like HgSe, HgTe, InAs, and PbX (X = S, Se, Te) NCs, are emerging as new promising class thanks to the easy production
process by colloidal synthetic methods in aqueous or organic solution and size-depending energy gap25–27.
Metal-oxide films, like WO3, MoO3, TiO2, Ta2O5, and Nb2O5, are another
class of inorganic NIR materials showing interesting properties like electrochromic behavior and, in reduced form, strong absorption in the NIR region28.
As regards the organic materials, typical NIR absorbing/emitting compounds are π-conjugated chromophores, like polyenes and polymethines29,30
, charge-transfer chromophores, like cyanines31,32 and azo dyes33,34, metal complexes like porphyrines35,36 and donor-acceptor chromophores37–39. The energy gap and consequently the optoelectronic properties of these compounds can be controlled through several factors, like bond length alternation and donor-acceptor charge transfer which will be discussed in the next section (1.2).
1.1.2. Application of NIR materials
The fluorescence, absorption, photoconductive, photosensitizing, photochromic and other properties of the NIR organic materials can find application in different military and civilian fields: military applications include target acquisition, surveillance, night vision, homing, and tracking, while civilian application include energy harvesting, bio-imagining, telecommunication40,41. NIR absorbing materials found application in different technological sectors: for example, they are used as pigmets in laser printers, but also as filter in plasma TV and photosensitizer in photodynamic therapy for treatment of cancer37,42.
In the last decades researchers focused on the synthesis of new material and or new design of solar cells in order to boost the power conversion efficiency (PCE)43,44. One way it is to use NIR sensitizer since more than 50% of solar radiation falls in the NIR spectral region45–47: the use of ternary ink (NIR
sensitizer, donor polymer and fullerene) has demonstrated to improve of more than 30% the performance compared to the same device without sensitizer48.
Figure 1. Solar energy distribution (Image courtesy of Heat Island Group, Lawrence Berkeley National Laboratory)
NIR organic emitters are less available, but are receiving more attention for their potential application in optical communication, NIR emissive organic materials may find applications in night-vision target identification, information security display, and sensors49.
As regards the bio imagining, NIR dyes show interesting feature like minimal interfering absorption and fluorescence from biological samples, inexpensive laser diode excitation, reduced scattering and enhanced tissue penetration depth50,51. Boppart et al.52 presented, for example, a new contrast-enhancing agent for tomography and more recently Li et al. presented a new imagining probe, emitting in the NIR region, for analysis in vivo.
1.2 Molecular design and energy gap engineering
The optical and electronic properties of organic materials depend on the energy gap, which is the difference between the highest occupied molecular orbital (HOMO) and the lowest unoccupied molecular orbital (LUMO). Lowering the energy gap results in a red shift of absorption and emission spectra, therefore the engineering of HOMO-LUMO level is a key for low energy gap materials and several design factors, as intrinsic energy gap, conjugation length and donor-acceptor charge transfer should be considered.
1.2.1 Intrinsic energy bandgap
In polyene, like polyacetylene, electrons can be delocalized, if there are no defects, all along the chain, while in polyarylene there is a competition between the delocalization of electrons along the chain and confinement in the rings; the resonance energy, is a measure of this delocalization and of monomer stability. Moreover in polyarylene system there are two ground states, corresponding at two limiting mesomeric forms obtained by the flip of the double bonds, which are not energetically equivalent. While the aromatic form is energetically more stable, the quinoid form has a higher energy but a lower energy gap53.
The intrinsic bandgap of an isolated conjugated polymer chain can be described by a combination of different energy contribution related to the bond length alternation (BLA), the resonance energy stabilization (RE), the torsional angle θ and the mesomeric or inductive effect of substituent (ER)
If we consider polyacetylene, we can describe it as infinite chain of CH, with a completely filled valence band and it should behave as a conductive metal, but between the valence band and the conduction band there is a forbidden zone (the energy gap) originated by the alternation of short (double) bond
and long (single) bond and described by the so called Peierls instability55. The value of the energy gap so, can be correlated to the degree of BLA, Δr, defined as length difference between a double and a single bond: the larger the Δr, the higher it will be the energy gap. In polyaromatic compound Δr is defined as maximum difference between the length of a C-C bond inclined relative to the chain axis and a C-C bond parallel to the chain axis. Bredes56,57 studied the relationship between Δr and energy gap in polythiophene and from theoretical calculation they found how Δr tends to be more positive when the quinoid contributions to RE increase (Figure 2).
Figure 2. Evolution of the bandgap Eg (eV) as a function of aromatic and quinoid
character. (Reproduced by permission of Elsevier Science from J. L. Bredas, Synth. Meth. 17,115 (1987). Copyright © 1987, Elsevier Science.)
This concept results in the synthesis of polyisothianaphtene by Kobayashi et al.58. Polyisothianaphtene is a polythiophene derivate where all thiophenes are fused with a benzene ring through β-β’ thiophene bond: the benzene rings stabilize the quionoid contributions and the energy gap decreases from 2.2 eV in polythiophene to 1.0 eV in polyisothianaphtene59.
Furthermore, the presence of heteroatoms in aromatic ring systems can considerably influence the electronic properties. The effect of such a substitution on the relative stability of aromatic ring systems can be evaluated by the resonance energy per electron (REPE). Table 1 shows the decrease of the energy gap upon decreasing the value of REPE. This means that decreasing the aromaticity of the polymer leads to lowering of the band gap it will be60,61.
Table 1. Resonance Energy (RE) and resonance energy per electron (REPE) values for various heterocyclic and the energies gap (eV) of corresponding polymers.
Not less important is the linearity of polymer chains for the delocalization of electrons along the π-system. Bredas et al. calculated62
, on theoretical level, the correlation between the energy gap and the torsional angle and found out that increasing the dihedral angle θ from 0° to 90° leads to an increase of the energy gap from a minimum value to a maximum, because of the cosθ dependence of π-orbital overlap. These results were confirmed also by Cui and Kertsets63 studying polythiophene: the bandgap is maximum, 4.5 eV, with θ = 90°, corresponding to no π-electron interaction between neighboring ring systems, and a further increase, from 90° to 180° results in a decrease of the bandgap; at 180°, in trans-coplanar conformation, the theoretical value of Eg is 1.7 eV.
Substituents play also a fundamental role in the bandgap engineering and their introduction is a direct way to modify the HOMO and LUMO energy levels and to fine tune the energy band gap.
Compound RE (β) REPE (β) Eg (eV)
Benzene 0.390 0.065 3.4
Pyrrole 0.233 0.039 3.1
Thiophene 0.193 0.032 2.1
Electron-withdrawing groups, such as nitro, carboxy or cyano and electron-donating groups such as alkyl, alkoxy or alkylsulfanyl have a mesomeric and/or inductive effect which stabilize the energy level and reduce the Eg.
The electron-withdrawing substituents down-shift the LUMO and HOMO energy levels versus vacuum (the down-shift of the LUMO is usually more than that of the HOMO), while electron-donating substituents upshift the LUMO and HOMO energy levels (the up-shift of the HOMO is usually more than that of the LUMO)64. For example the introduction of an electron-withdrawing group such as a cyano in the vinylene linkage in poly(thienylenevinylene) results in a decrease of LUMO level due to the inductive effect (-I) of cyano group and a general reduction of energy gap (from 1.80 eV to 0.60 eV)65.
We can say that all of the factors leading to a decrease in π-delocalization across the polymer backbone will result in an increasing in the bandgap and vice versa.
1.2.2 Effect of conjugation length and aggregation
The extension of conjugation length in conjugated systems results in a decrease, to some extent, of the energy gap. The conjugation can be increased in a linear 1-dimensional elongation by linking covalently or fusing π-conjugated units, like, for example, in polythiophene66
, poly(para-phenylene)67 and rylenediimides oligomers68.
Theoretical calculations clearly show how adding thiophene units decrease the energy gap and, for the rylenediimides, the increase of the degree of annulation by going from perylenediimide to hexarylenediimide leads to a gradual bathochromic shift of the absorption maximum, with an energy gap going form 2.15 eV to 1.25 eV.
Anyway the energy gap of a conjugated system can be lowered by increasing π-conjugation only until a limit point, since the whole system is governed by the effective conjugation length69.
Inter-molecular effects and aggregation in solid state also play an important role on influencing the energy gap: strong interaction and formation of H- and J- aggregates influence the optoelectronic characteristic such as absorption and charge mobility70–72.
1.2.3 Donor-Acceptor Approach
A different approach for tuning the energy levels is the use of alternating donor-like (electron donating) and acceptor-like (electron withdrawing) monomers73,74. In these systems, called push-pull, the hybridization of energy levels of donor and acceptor increases the HOMO level so that it becomes higher than the one of donor and decreases the LUMO lower than that of the acceptor (Figure 3): the results is a small HOMO-LUMO gap.
Figure 3. Hybridization of frontier molecular orbitals (HOMO and LUMO) of donor and acceptor units to yield a low bandgap D–A monomer unit.
Depending on the strength of the donor and acceptor monomer, the energy gap can be fine-tuned: in order to get close HOMO LUMO levels, strong acceptor, such as benzothiadiazole and benzobisthiadiazole, and strong donor, such as thienothiophene and benzodithiophene can be used. An important role plays also the spacer linking the donor and acceptor, which can influence the hybridization and as consequence the energy gap75.
1.3 BODIPY dyes
4,4-Difluoro-4-bora-3a,4a-diaza-s-indacene dyes, more commonly known as BODIPY dyes, have been long since recognized for their excellent optical properties such as high absorption coefficients, high fluorescence quantum
yields, and remarkable photostability76. Discovered for the first time in 1968 by Treibs and Kreuz77, BODIPY dyes are of wide importance and have a broad use as laser dyes in biological sensing, organic electronic, and other possible applications78–87. Additionally, straightforward chemical synthesis and structural robustness have enabled fine tuning of optical properties of BODIPY dyes via systematic structural variations78,83. The absorption and fluorescence properties depend on the position of substitution (Figure 4), where addition of an electron donating substituent to position 8 does not cause a substantial change of the photophysical behaviour88, but bulky electron donating groups in positions 2 and 6 cause a large red shift in the absorbance and fluorescence. The effect of an electron withdrawing group is different, with a red shift of the absorbance and fluorescence with addition of the electron withdrawing unit, like a cyano group, to position 8. Addition of a cyano group to positions 2 and 6 causes a smaller change of absorbance and fluorescence wavelength, but it may have a large effect on the fluorescence quantum yield. The presence of bromine atoms in positions 2 and 6 also does not have a substantial effect on the absorbance and fluorescence wavelength89. Formation of conjugated systems via positions 2 and 6 also has an effect on the photophysical properties of the BODIPY dyes, showing red-shifted behavior with an increasing degree of conjugation90,91. BODIPY compounds blocked by alkyl or aromatic groups show one-electron Nernstian reduction and oxidation waves for the first electron transfer, where the chemical reversibility depends on the character of substitution92,93. The stability of anion radicals depends on substitution in position 8, which is subject to nucleophilic attack, while the cation radicals are stabilized by substitution at the 2 and 6 positions, preventing electrophilic attack. Conjugated polymers with on chain BODIPY as well as the corresponding 4-bora-3a,4a,8-triazaindacene core (Aza-BODIPY) can potentially extend the absorption into the deep-red regions of the visible
spectrum and, in some cases, are excellent near-infrared emitters. Aza-BODIPY dyes (Figure 4) contain a nitrogen in the meso (8) position which appears to reduce the HOMO-LUMO energy gap relative to BODIPY dyes bearing similar substituents. The relatively high extinction coefficients of these polymers combined with their photostability make them attractive candidates for various optoelectronic applications
Figure 4. General Chemical Structure of BODIPY and Aza-BODIPY .
As outlined before, in recent years, researchers have showed great interest in low band gap (LBG) organic materials that absorb into the near-infrared (NIR). Even though semiconducting polymers with ultra LBGs have been synthesized before, the design and synthesis of materials with good photoresponse beyond 900 nm and an appreciable PCE in polymer:fullerene solar cells is still a challenge. The key for the design of this polymer is the precise energy level control. The fine tune of energy band gap can be obtained with the donor-acceptor (D-A) approach or the stabilization of aromatic-quinoid structure. D-A approach is the most common tool to synthesize NIR conjugated polymers due to the great amount of functional electron rich and electron deficient building blocks. In order to develop ultra LBG D-A polymers, usually strong electron rich units, like pyrrole, thiophene, ethylenedioxythiophene (EDOT), or bridged bithiophene derivatives and strong electron deficient building blocks, like benzobisthiadiazole, diketopyrrolopyrrole dyes, pyrazinoquinoxaline
derivatives, thiadiazoloquinoxaline derivatives, thienoisoindigo, emeraldicene, or tetraazabenzodifluoranthenediimide are used.
BODIPY small molecules have been recently employed as p-type or donor materials in conjunction with PCBM in bulk heterojunction (BHJ) solar cells thanks to the large extinction coefficients, intense absorption spectra that extend into the red region of the visible spectrum, and decent hole mobility. Also BODIPY-based conjugated polymers have been used in different applications, such as near- IR emitters, light harvesting and OPVs, but only few examples of ultra LBG conjugated polymers (Eg < 1.4-1.5 eV) with
BODIPY core have been presented. Actually, Algi and Cihaner designed and synthesized a BODIPY-based polymer for electrochromic applications. In their study, a 1,3,5,7-tetramethyl substituted BODIPY derivative was used as an acceptor unit, featuring a non-planar repeating unit and distorted conjugation between EDOT (strong electron rich) and BODIPY (electron deficient) units due to the steric effect of the methyl groups. To avoid the steric effect of the methyl groups, Vobecka et al.94 and Samuel et al.95 have synthesized a BODIPY core with halogens at 3- and 5- positions (α-positions) and effectively synthesized an EDOT-BODIPY-EDOT conjugated polymer both with electro-polymerization and Stille cross coupling polymerization, respectively. However, the resulting copolymers are kinked because the linearity of the polymer was lost. Very recently, Stoddart et al96. succeeded to synthesize the first ultra LBG DAD type α,β-unsubstituted BODIPY-based copolymer using EDOT as the electron rich (D) unit by electro-polymerization which displays electrochromic behavior.
During the PhD thesis, new LBG conjugated polymers and small molecules based on α,β-unsubstituted BODIPY core monomers have been designed and effectively synthesized by conventional cross coupling reaction such as Stille and/or Suzuki coupling.
2. BODIPY Polymers
2.1 Cross-coupling reactions for the synthesis of BODIPY-based polymers and small molecules
The structure of BODIPY is commonly described as being a boradiazaindacene by analogy with the all-carbon tricyclic ring, but can be also regarded as a cross-conjugated cyanine. The starting point for the synthesis of symmetric (Scheme 1) and asymmetric (Scheme 2) BODIPY unit is the condensation reaction between a highly electrophilic carbonyl compound like an aldehyde and pyrrole, forming a bridge between two pyrrole, followed by oxidation with p-chloranil or dichloro-dicyano-quinone (DDQ) and complexation with boron trifluoride diethyletherate catalyzed by a base (usually a tertiary amine).
Scheme 1. Synthetic pathway for symmetric BODIPY.
The BODIPY and aza-BODIPY can be easily modified introducing halogen atom with electrophilic substitution reactions (introduce halogen mainly in 2 and 6 positions) (Scheme 3) or using halogenated dipyrromethene precursors (Scheme 4).
Scheme 3. Halogenation of BODIPY core by electrophilic substitution.
Scheme 4. Halogenation of BODIPY starting from halogenated precursors.
The halogenation of BODIPY in α or β positions open many possibilities not only in the field of small molecule semiconductors38, but also in the polymers one. The halogenated BODIPYs will be suitable to undergo nickel-catalyzed cross coupling polymerization reaction such as Yamamoto coupling as well as palladium-catalyzed cross coupling reactions, like Sonogashira, Heck, Stille or Suzuki coupling (Scheme 5)97, facilitating the extension of π-conjugation length and building more complex structures.
Scheme 5. Nickel and Palladium-catalyzed cross coupling reaction suitable for halogenated BODIPY core.
In this chapter, the synthesis and the optoelectronic characterization of novel ultra LBG polymers consisting of α,β-unsubstituted meso positioning BODIPY as building block are presented (Figure 5).
Figure 5. α,β-unsubstituted meso positioning BODIPY-based polymers.
2.2 Results and discussion
2.2.1. Theoretical calculations
The development of BODIPY-based organic semiconductors and especially those of the α,β-unsubstituted forms has so far lagged behind that of other π-deficient units, mainly because of stability issues during the synthesis. However, thanks to a recently developed synthetic protocol37, a stable α,β-unsubstituted BODIPY functionalized solely on the meso position with a thienyl group has been successfully synthesized (Scheme 8) and integrated into more complex structures. The structural and electronic properties of the recently developed building block along with its structural analogues containing dimethyl substituents at the α-positions and tetramethyl substituents at the α,β-positions were determined via quantum chemical density functional theory (DFT) calculations utilizing the
311G(d,p) as the model basis set and the results are presented in Figure 6. As shown in Figure 6, on the one hand the π-electron density of the highest occupied molecular orbital energy level (EHOMO) of all the three studied
BODIPY monomers is found to be delocalized only on the dipyrromethene core (without the participation of the N-B(F2)-N sequence) along with the methyl groups in the case of the α-substituted meso-positioning thienyl BODIPY and the α,β-substituted meso-positioning thienyl BODIPY. On the other hand, the π-electron density of the lowest unoccupied molecular orbital energy level (ELUMO) is not only distributed throughout the
boron-dipyrromethene core but is also found to be extended towards the meso-thienyl unit as the methyl substitution decreases. In addition, it is evident that as the number of the methyl substituents decreases both the EHOMO and
ELUMO levels are downshifted vs vacuum due to the elimination of the
σ-inductive effect of the methyl groups, but no significant variation is detected on the calculated EHOMO-ELUMO gap. Furthermore, the subsequent exclusion
of the methyl substituents from the α- and β-positions leads to the reduction of the dihedral angle between the boron dipyrromethene core and the meso-thienyl unit from 89.8o for the α,β-substituted meso-positioning thienyl BODIPY to 50.7o for the α-substituted meso-positioning thienyl BODIPY and finally to 47.3o for the α,β-unsubstituted meso-positioning thienyl BODIPY. The reduction of the dihedral angle, especially in the α,β-unsubstituted meso-positioning thienyl BODIPY, could contribute to the efficient π-π stacking and C-H…π interactions when this building block would be integrated into π-conjugated polymer backbones.
Figure 6. Calculated frontier molecular orbital (EHOMO/ELUMO) levels, molecular dipole
moments (μ), dihedral angles between the boron dipyrromethene core with the thienyl ring and pictorial representations of the model monomers α,β-unsubstituted meso-positioning thienyl BODIPY, α-substituted meso-meso-positioning thienyl BODIPY and the α,β-substituted meso-positioning thienyl BODIPY (B3LYP/6-311G(d,p) level of theory).
The dipole moment (μ) of the α,β-unsubstituted meso-positioning thienyl BODIPY (6.54 D) is higher than those of the α-substituted BODIPY (4.86 D) and the α,β-substituted BODIPY (5.07 D). The μ of the α,β-unsubstituted meso-positioning thienyl BODIPY (6.54 D) is higher than that of the α,β-substituted BODIPY (5.07 D) due to the absence of the methyl groups that decrease the electron affinity of the BODIPY core through their σ-inductive effect. In addition, the symmetric α,β-unsubstituted and α,β-substituted meso-positioning thienyl BODIPY monomers present higher μ than the asymmetric α-substituted BODIPY (4.86 D). Therefore, the higher μ value of the α,β-unsubstituted meso-positioning thienyl BODIPY is expected to enhance the backbone-ordering and as a consequence the crystallinity of the
corresponding π-conjugated polymer thin films as a result of strong dipolar interactions52.
2.2.2. Synthesis of α,β-unsubstituted meso positioning BODIPY precursors
The easiest way to synthesize α,β-unsubstituted BODIPY dyes is the combination of aldehydes and pyrrole under neat conditions. The aldehyde can be dissolved in excess pyrrole at room temperature, and the dipyrromethane intermediate (the reduced form of the dipyrromethene) is formed and isolated. The BODIPY core can then be obtained after oxidation and complexation with boron. During the PhD thesis, 5-octylthiophene-2-carbaldehyde has been chosen as the aldehyde, and upon condensation with pyrrole, catalyzed by few drops of trifluoroacetic acid, the resulting 2,2'-((5-octylthiophen-2-yl)methylene)bis(1H-pyrrole) (1) is obtained (Scheme 6).
Scheme 6. Synthesis of 2'-((5-octylthiophen-2-yl)methylene)bis(1H-pyrrole).
We decided to choose alkylthiophene-carbaldehyde in order to have the formation of a functional BODIPY building block (3) with a 2D extension for the development of a series of BODIPY based copolymers soluble in common organic solvents. Treatment of monomer 1 with the strong oxidant
2,3-dichloro-5,6-dicyano-1,4-benzoquinone (DDQ), then
diisopropylethylamine (Hünig’s base) and finally with trifluoroborane dietherate [BF3O(Et)2] provided the corresponding borondipyrromethene
Scheme 7. Synthesis of 8-octylthiophene BODIPY.
New protocols to introduce bromine in 2- and-6 positions on the unsubstituted BODIPY core has been presented in the literature by Shinokubo et al.98 and Zhang et al.99 In our case, the targeted dibromo borondipyrromethene monomer 3 is synthesized upon bromination with N-bromosuccinimide (NBS) using dimethylformamide (DMF):methylene chloride (CH2Cl2) 1:1 as the solvent mixture similar to the conditions
presented by Stoddart et al.96 (Scheme 8).
Scheme 8. Synthesis of 2,6-dibromo-8-octylthiophene BODIPY.
Then, Stille cross coupling reaction between monomer 3 and the commercial
avaible 2-(tributylstannyl)thiophene using as catalyst
tris(dibenzylideneacetone)dipalladium(0) [Pd2(dba)3] and
tri-o-tolylphosphine [P(o-Tol)3] in inert atmosphere and dry toluene provide
monomer 4 (Scheme 9). The purified monomer 4 then was brominated, following a classical protocol, with NBS in DMF, in order to provide the functional monomer 5 (Scheme 9).
Scheme 9. Synthesis of monomer 5.
2.2.3 Synthesis of polymers 126.96.36.199 Synthesis of TBDPTV
TBDPTV was synthesiszed through Stille cross-coupling polymerization using 1:1 monomer feed ratios (Scheme 10). A solution of the commercially available (E)-1,2-bis(3-dodecyl-5-(trimethylstannyl)thiophen-2-yl)ethene and the dibromo borondipyrromethene monomer 3 were combined in dry deoxygenated toluene in the presence of Pd2(dba)3 (5 mol%) and P(o-Tol)3
(40 mol%) and the mixture was heated to ca. 120°C for 48 h to provide the desired crude polymer. Purification was achieved by Soxhlet extraction with methanol (200 mL, 1 d), hexane (200 mL, 1 d) and chloroform (200 mL, 1 d). The chloroform fraction was then concentrated under reduced pressure, precipitated in methanol, filtered and dried in vacuum. Polymer TBDPTV is readily soluble in chloroform, chlorobenzene and o-dichlorobenzene (o-DCB). The typical molecular weight characteristics of TBDPTV were estimated by GPC and are presented in Table 2.
Scheme 10. Synthesis of TBDPTV.
188.8.131.52 Synthesis of BODIPY-qTo and BODIPY-qTi and CB06
Stille coupling mediated polymerisation ([Pd2(dba)3] (2 mol %), [P(o-tol)3]
(4 mol %) in toluene at ca. 120 °C for 48 h) was used to combine the BODIPY precursor 5 (Figure 6) with readily available (3,3'-didodecyl-2,2'-bithiophene-5,5'-diyl)bis(trimethylstannane) or (4,4'-didodecyl-2,2'-bithiophene-5,5'-diyl)bis(trimethylstannane) or (E)-1,2- bis(3-dodecyl-5-(trimethylstannyl)thiophen-2-yl)ethene to provide the polymers BODIPY-qTo, BODIPY-qTi and CB06, respectively (Scheme 11).
The crude polymers as received from the reaction mixtures were purified by successive Soxhlet extractions and they were collected by precipitation from the chloroform (CF) fraction (BODIPY-qTo) and chlorobenzene (CB) fraction (BODIPY-qTi, CB06). The resulting polymers are soluble in chloroform, chlorobenzene and o-dichlorobenzene (o-DCB). The average molecular weights ̅̅̅̅, ̅̅̅̅ and the polydispersity (Đ) of the polymers were measured by GPC based on monodispersed polystyrene standards at high temperature (150 °C) with 1,2-dichlorobenzene (DCB) as eluent for BODIPY-qTo and BODIPY-qTi, while the GPC analysis for CB06 was performed at 30°C using chloroform as eluent (Table 2). Both BODIPY-qTo and BODIPY-qTi show monomodal GPC profiles with no appearance of residual monomers or oligomer chains. BODIPY-qTo exhibits ̅̅̅̅ of 72000 g/mol, with Đ of 1.57, which is significantly higher than that of BODIPY-qTi ( ̅̅̅̅ = 22400 g/mol, with Đ = 1.74). Since that BODIPY-qTi is received from the CB fraction it seems that anchoring the didodecyl side chains on the i-positions prevent the easy solubility of the polymer chains in common organic solvents, which could explain the lower ̅̅̅̅ of BODIPY-qTi.
Table 2. Molecular Characteristics of TBDPTV, BODIPY-qTo, BODIPY-qTi and CB06.
Polymer Mn (g/mol) Mw (g/mol) Đ Polymerization
TBDPTV 13700 70300 5.1 15
BODIPY-qTo 72000 113000 1.6 69
BODIPY-qTi 22400 40000 1.7 21
2.2.4 Electrochemical Characterization
The energy levels of TBDPTV have been determined with both cyclic voltammetry (CV) and atmospheric pressure photoelectron spectroscopy (AAPPS) (Figures 7 and 8).
Figure 7. Cyclic voltammogram of TBDPTV in chloroform (containing 0.1 M tetrabutylammonium perchlorate).
Figure 8. HOMO energy level of TBDPTV estimated by atmospheric pressure photoelectron spectroscopy.
The reduction and oxidation versus saturated calomel electrode (SCE) of TBDPTV are, respectively, at -0.68 V and 0.46 V (Figure 7). The resulting
HOMO (EHOMO) and LUMO (ELUMO) energy levels as calculated from the
equations EHOMO = -(4.7 + Eonset ox
) eV and ELUMO = -(4.7 + Eonset red
) eV are -5.16 eV and -4.02 eV vs. vacuum, respectively. The electrochemical bandgap (Eg
) of 1.14 eV is in excellent agreement with the Eg opt
(Table 3 at page 27). The HOMO level as calculated by AAPPS is situated at -5.29 eV, slightly different from the one obtained by cyclic voltammetry.
Also for BODIPY-qTi and BODIPY-qTo, cyclic voltammetry has been performed (Figure 9). Both BODIPY-qTi and BODIPY-qTo exhibit reversible oxidation and reduction peaks. It is demonstrated that the oxidation and reduction potentials of the polymers are alkyl side chain positioning dependent.
Figure 9. BODIPY-qTi, BODIPY-qTo and PC71BM cyclic voltammetry graphs during oxidation (left) and reduction (right).
BODIPY-qTi and BODIPY-qTo present oxidation/reduction potentials at 0.62 V/-0.63 V vs saturated calomel electrode (SCE) the former and at 0.69 V/-0.61 V vs SCE the latter. These lead to EHOMO/ELUMO levels at -5.32
eV/-4.07 eV for the BODIPY-qTi and at -5.39 eV/-4.09 eV for the BODIPY-qTo vs vacuum resulting to very low Eg
of 1.25 eV for the BODIPY-qTi and of 1.30 eV for the BODIPY-qTo. The obtained Eg
of the polymers are increased by 0.05 eV than their corresponding Eg
(Table 3) in agreement with recently reported results on other polymer systems100. It is obvious that when the didodecyl side chains are anchored onto the tail-to-tail (TT) positioning both the EHOMO/ELUMO levels are upshifted as compared to
BODIPY-qTo. A tentative explanation for the lower lying EHOMO/ELUMO
levels of BODIPY-qTo can be attributed to the steric constraints that prevent planarity of the quaterthiophene segment when the didodecyl alkyl chains of the two central thiophene units are anchored in the head-to-head (HH) positioning. For comparison the reduction potentials of the well-known organic semiconductor fullerene derivative [6,6]-phenyl-C71-butyric acid
methylester (PC71BM) with strong electron withdrawing characteristics have
also been determined by CV. PC71BM presents three reversible reduction
peaks at -0.68 V, -1.06 V and -1.56 V vs SCE that are attributed to ELUMO
(-4.02 eV), ELUMO+1 (-3.64 eV) and ELUMO+2 (-3.14 eV), respectively. These
results show that the ELUMO levels of BODIPYqTi and BODIPY-qTo are
lying lower by 0.05 eV (BODIPY-qTi) and 0.07 eV (BODIPY-qTo) as compared to PC71BM. The combined low ELUMO levels and small bandgaps
and Eg opt
) are indicative of the highly electron-deficient and π-conjugated nature of the α,β-unsubstituted meso-positioning thienyl BODIPY. These are among the lowest ELUMO levels reported to date for a
semiconducting polymer comparable to those of the 2,2′-(bisindenofluorene-12,15-diylidene) dimalononitrile-based quaterthiophenes101,102 and
approaching those of air-stable n-channel core-cyanated perylene-, anthracene- and naphthalene-based small molecule semiconductors103–105. Figure 10 show the predicted EHOMO and ELUMO levels as well as the
distribution of the frontier molecular orbitals of the BODIPY-qTi and BODIPY-qTo.
Figure 10. Schematic illustration of the calculated frontier molecular orbital EHOMO
(orange band) and ELUMO (blue band) levels variation and pictorial representations of the
trimer model compounds BODIPY-qTi and BODIPY-qTo (B3LYP/6-311G(d,p) level of theory) and with black lines the experimentally determined EHOMO/ELUMO levels of
BODIPY-qTi, BODIPY-qTo and PC71BM.
It is possible to observe that in BODIPY-qTi and BODIPY-qTo the EHOMO
levels are fully delocalized along the polymer chain axis in contrast to the significant localization of the ELUMO on the α,β-unsubstituted
meso-positioning thienyl BODIPY along with a good agreement in the variation between the theoretically predicted and the experimentally determined EHOMO and ELUMO levels.
2.2.5 Optical Characterization
The normalized UV–vis absorption spectra of TBDPTV, CB06, BODIPY-qTo and BODIPY-qTi in chloroform solution and in the solid state were measured and presented in Figures 11-13, whereas the corresponding optical
properties are summarized in Table 3. All the polymers show two major absorption bands, both in solution and in solid state, a feature commonly observed for alternating D-A copolymers. The low-wavelength peak observed can be attributed to a π-π* transition, while the high-wavelength transition with is believed to be related to an intramolecular charge transfer (ICT) between the electron donating and the electron deficient groups of the repeating unit. Focusing on TBDPTV (Figure 11), by passing from solution to the solid state, the absorption spectrum becomes broader covering all the range from 300 nm to 1100 nm and all the absorption bands are redshifted. The peak at 444 nm in solution is situated at 451 nm in the solid state, whereas the peak at 817 nm in solution has been shifted to 848 nm in the solid state, indicating the presence of strong intermolecular π-π interactions. The optical band gap (Eg
) calculated from the absorption onset in the solid state is estimated at 1.15 eV.
Table 3. Absorption maxima and energy gap of polymers TBDPTV, BODIPY-qTo, BODIPY-qTi and CB06.
Polymer λmaxsol (nm) λmaxfilm (nm) Egopt (eV)
TBDPTV 444, 817 451, 848 1.15
BODIPY-qTo 424, 715 415, 739 0.98
BODIPY-qTi 426, 739 446, 782, 877 0.85
Figure 11. UV-vis Absorption spectra in chloroform solution and as thin film of TBDPTV.
The chemical structure of CB06 is similar as to TBDPTV, but with one more thiophene unit between the BODIPY and the bis(3-dodecyl-thiophen-2-yl)ethene. Compared to TBDPTV, CB06 absorption maxima, both in solution (462 nm and 762 nm) and solid state (484 nm and 794 nm), on the one hand is red shifted at the low wavelength band as a result of the extension of the π-conjugation along the polymer backbone induced by one more thiophene. On the other hand, the high wavelength band is blue shifted in agreement with the finding from a recent work106 in which it is reported that the stronger the coupling between the D and A moieties or the shorter the conjugation length between two electron withdrawing units within the polymer chain, the higher is the wavelength of the maximum absorption. The estimated Eg
Figure 12. UV-vis spectra of CB06 in chloroform solution and as thin film.
BODIPY-qTi and BODIPY-qTo show qualitatively similar spectral shape with two well resolved vibronic transitions (Figure 13). The low-wavelength peak observed at 426 nm for BODIPY-qTi and at 424 nm for BODIPY-qTo can be attributed to the polymers backbone π-π* transition while the high-wavelength transition at 739 nm for BODIPY-qTi and at 715 nm for BODIPY-qTo is related to an intramolecular D-A charge transfer excitation.
Figure 13. UV-vis spectra of BODIPY-qTi and BODIPY-qTo polymers in chloroform solution and as films.
Polymer BODIPY-qTi presents two additional low absorption bands between 1600 and 1800 nm. This absorption peaks could be attributed to some weak electronic transitions from interchain interactions but more experiments and studies are needed to support this assumption.
Passing from solution to the solid state, both the low- and high- wavelength absorption peaks of BODIPY-qTi and BODIPY-qTo are red shifted with respect to their solution spectra, except for the low wavelength absorption peak of BODIPY-qTo (Table 3). This supports the efficient π-π stacking of the polymer chains of BODIPY-qTi passing from solution to the solid state. In general, the same trends observed in solution for the BODIPY-qTi and BODIPY-qTo regarding the variation of the absorption maxima of both the low and high wavelength peaks were also observed in the solid state studies (446/782 nm for BODIPY-qTi and 415/739 nm for BODIPY-qTo). However, BODIPY-qTi reveals a pronounced absorption peak at longer wavelength (877 nm), a signature of a vibronic feature which denotes enhanced aggregate formation similar to that observed in regioregular poly(3-hexylthiophene) thin films, indicating a more ordered structure.55 Furthermore, the Eg
of BODIPY-qTi and BODIPY-qTo (Table 3) support that these polymers are ultra LBG polymeric semiconductors. The Eg
of BODIPY-qTi (0.85 eV) is lower by 0.13 eV than that of BODIPY-qTo (0.98 eV). Therefore, when the didodecyl side chains are anchored onto the HH positions in BODIPY-qTo the absorption peak maxima both in solution and in solid state appear at lower wavelengths and the Eg
is higher as compared to BODIPY-qTi, indicating a higher degree of steric hindrance and polymer chain distortion.
To support our assumption quantum chemical DFT calculations were performed to estimate the dihedral angles, predict the molecular energy levels and model the distribution of the frontier molecular orbitals of the BODIPY-qTi and BODIPY-qTo. The DFT calculations using the
311G(d,p) performed on trimer model compounds and the chemical structures of the BODIPY-qTi and BODIPY-qTo as obtained by the theoretical calculations are presented in Figure 14 and the estimated dihedral angles in Table 4.
Figure 14. Ground state geometry optimizations of BODIPY-qTi and BODIPY-qTo. Color scheme: carbon, gray; nitrogen, blue; sulfur, orange; boron, pink; fluorine, cyan. Optimized structures calculated using DFT at the B3LYP/6-311G(d,p) level of theory. θ1,
θ2, θ3, θ4 and θ5 are the calculated dihedral angles.
Table 4 Calculated dihedral angles (θ1, θ2, θ3, θ4 and θ5) of some representative bonds that are shown in Figure 14 for BODIPY-qTi and BODIPY-qTo polymers.
θ1 θ2 θ3 θ4 θ5
BODIPY-qTi 33.2o 20.9o 30.5o 18.1o 16.8o BODIPY-qTo 23.8o 63.4o 21.4o 19.2o 20.1o
The obtained results show that BODIPY-qTi and BODIPY-qTo present comparable estimated dihedral angles except in the case of θ2 dihedral angle
where the rotation between the adjacent units in BODIPY-qTo is 63.4° as compared to 20.9° in BODIPY-qTi. The lower θ2 dihedral angle between the
adjacent didodecyl thiophene rings of BODIPY-qTi results in reduced steric hindrance along the axis when the didodecyl alkyl chains are anchored in the i-positions, which is beneficial towards enhanced optoelectronic and charge transporting properties107,108. These findings are in agreement with the aforementioned observation on the absorption maxima and Eg
variation for BODIPY-qTi and BODIPY-qTo.
The research group of Dr. Stratakis from IESL, Heraklion Crete, has performed also the micro-photoluminescence (μPL) measurements. μPL experiment is a photoluminescence experiment with spatial resolution and it allows to study any nanostructures and/or defects and in our case to examine if the studied polymer thin films present any type of aggregation (ordering). The spectra of both polymers are presented in Figure 15 .
Figure 15. Room temperature μPL spectra following excitation at 543 nm of the BODIPY-qTo (black line) and BODIPY-qTi (red line) polymers.
While it is possible to observe significant quenching (~20%) for the BODIPY-qTi polymer relative to the BODIPY-qTo one, no significant μPL peak shift is noticed. This finding is rationalized if one considers the better
π-π stacking of the BODIPY-qTi polymer chains due to the reduced steric hindrance as compared to the BODIPY-qTo. Notably, the sharp peak at ca. 590 nm (2.1 eV) corresponds to the Raman signature of the symmetric vibration, νs(C=C), of the carbon-carbon double bond within the thiophene
ring at 1450 cm-1.
The pristine polymers BODIPY-qTo and BODIPY-qTi were also studied by means of transient absorption spectroscopy (TAS) in order to examine the photo-excitation dynamic processes that occur following 1026 nm laser excitation. It is worth to mention that at least two-photon absorption is used in order to excite these polymers, because the energy of the employed fundamental wavelength, i.e. 1026 nm, is lower than the energy an electron needs to move from the EHOMO to ELUMO of the polymers in question. Figures
16a and 16b present the normalized delta optical density (ΔOD) vs. wavelength, for the two polymers studied (BODIPY-qTo and BODIPY-qTi) as a function of time, i.e. following photo-excitation at t=0 fs.
Figure 16. Normalized optical density vs. wavelength plots at various time delays of BODIPY-qTo (a) and BODIPY-qTi (b), following photo-excitation at 1026 nm with a pump fluence of 1.5 mJ cm-2.
For both polymers the transient photo-induced absorption (ΔOD) peak shifts to higher wavelengths, i.e. lower energies, as time progresses. Namely, within 200 fs, the BODIPY-qTo polymer peak shifts from 550 to 663 nm,
while the corresponding peak of BODIPY-qTi polymer shifts from 550 to 646 nm. This ultrafast red shift in both polymers is attributed to temporal post photo-excitation phenomena such as thermalization of the electrons and holes to the edge of the conduction and valence band, as well as, to the internal vibrational and rotational relaxations within the excited states.
2.2.6 Charge Transporting Properties of qTo and BODIPY-qTi
The research group of Prof. Thomas Anthopoulos from Imperial College has investigated the charge transport properties of qTo and BODIPY-qTi polymers in thin-film transistor devices. Initial measurements were performed using a bottom-contact (BC), top-gate device configuration with gold (Au) source-drain electrodes. Polymer films were cast by spin-coating and subsequently annealed at 100 °C before the deposition of the fluorinated ether (Cytop) gate dielectric. Both polymers exhibited p-type behaviour but significant differences were observed in their performance. Hence the transfer and output characteristics of BODIPY-qTi (Figures 17a,b) exhibited little hysteresis between the forward and reverse sweeps, with a threshold voltage around -15V. The saturated charge carrier mobility was relatively modest, around 5×10-4 cm2V-1s-1 (Figure 17c).
Figure 17. Transfer (a), output (b) characteristics of BC/TG configuration OFET device and mobility calculation based on first derivative of the linear regime transfer curve and first derivative of the square root of the saturation regime transfer curve (c) for the with BODIPY-qTi.
In contrast, devices of BODIPY-qTo exhibited significant hysteresis between the forward and reverse sweeps, with a much higher threshold voltage of around -50 V (Figure 18). The poor device characteristics made it difficult to extract robust mobility values, although they were approximately one order of magnitude lower than BODIPY-qTi .
Figure 18. Transfer (a), output (b) characteristics of BC/TG configuration OFET device and mobility calculation based on first derivative of the linear regime transfer curve and first derivative of the square root of the saturation regime transfer curve (c) for the BODIPY-qTo.
The reduced performance is likely due to a combination of the HH alkyl chains causing a large torsional twist in the conjugated backbone, inhibiting the close packing of the polymer chains, as well as the resulting increase in the ionisation potential, which increases the injection barrier.
Table 5. Summary of the FET performance of BODIPY-qTi and BODIPY-qTo polymers.
Polymer µ sat average (µ sat max) (cm 2 V -1 s -1 ) µ lin average (cm 2 V -1 s -1 ) V Th (V) Ion/Ioff BODIPY-qTi 4.7×10 -4 ± 3.1×10 -5 (4.9×10 -4 ) 3.5×10 -4 ± 3.8×10 -5 -14.4 ± 0.6 102-103 BODIPY-qTo 10-5-10-4 10-5-10-4 < -50 V 10-102
Despite the low-lying LUMO of both polymers, no obvious evidence for electron transport was observed in these devices. In order to improve the electron injection, the Au source/drain electrodes were replaced with Al in an otherwise identical device configuration, since the latter has a lower work function that could potentially facilitate electron injection from the metal to the semiconductor due to the reduced barrier. Despite the improvement and the matching electrode/ELUMO interface energetics, no electron accumulation
could be observed. Since the nature of the dielectric/semiconductor interface is also known to have a dramatic influence on the electron transport across the channel, top-contact, bottom-gate devices were fabricated using the divinyltetramethyldisiloxane-bis-benzocyclobutene (BCB) as the gate dielectric since the latter is known to provide an excellent interface with various high electron mobility organic semiconductors112–114. Control devices using the fullerene derivative [6,6]-phenyl-C61-butyric acid methyl ester
(PC61BM) as the semiconductor were also prepared in the same device
configuration. The latter samples demonstrated the expected transistor performance and in accordance with previously published data. However, we were unable to observe electron transport in either of the polymer devices (Figure 19).
Figure 19. Transfer curves of BG/TC configuration OFET device of (a) BODIPY-qTi and (b) BODIPY-qTo.
We therefore conclude that despite the low lying ELUMO, neither of the
polymers is a good electron transporting material. We believe this may be related to the poor delocalization of the ELUMO along the polymer backbone.
2.2.7 Photovoltaic properties of polymer TBDPTV
Among the synthesized polymers, TBDPTV showed the lowest optical energy gap and upshifted ELUMO level as compared to BODIPY-qTi and
material in bulk heterojunction (BHJ) solar cells. The research groups of Prof. Brabec from FAU University has tested it.
Organic BHJ solar cells were fabricated in inverted device structure consisting of ITO/ZnO/TBDPTV:PC71BM/MoOx/Ag, using three different
D:A composition ratio (1:2, 1:3 and 1:4). The active layer solution was spin coated under inert atmosphere condition using 97 to 3 vol % of chlorobenzene (CB) and 1,8 diiodooctane (DIO). Figures 20a,b show the J-V curves of the optimized BHJ solar cells under simulated AM 1.5G solar irradiance (100mW cm-2) and in the dark, respectively.
Figure 60. Current density-voltage characteristics under 100 mW cm-2 illumination (AM1.5G) (a) in linear graph and (b) in semilogarithmic graph.
The photovoltaic parameters obtained with the three different D:A ratio are summarized in Table 6.
Table 6. Photovoltaic parameters of TBDPTV:PC71BM system in different composition
ratio. TBDPTV:PC71BM Voc (V) Jsc(mAcm-2) FF (%) η (%) 1:2 0.58 (0.58 ± 0.00) 3.32 (3.27 ± 0.32) 53.45 (51.54 ± 1.82) 1.03 (0.97 ± 0.04) 1:3 0.59 (0.59 ± 0.00) 3.39 (3.16 ± 0.17) 56.18 (55.52 ± 0.58) 1.10 (1.03 ± 0.06) 1:4 0.59 (0.59 ± 0.00) 3.12 (2.86 ± 0.24) 56.51 (56.14 ± 0.37) 1.01 (0.93 ± 0.07)
A PCE of 1.1% was obtained for the 1:3 ratio, with a short circuit current density (Jsc) of 3.39 mA cm-2, Voc of 0.59 V and FF of 0.56. Using the same
fabrication conditions, solar cells containing 1:2 and 1:4 D:A ratio achieved a maximum efficiency of 1.03 and 1.01, respectively. A strong correlation between the charge carrier mobility and FFs is also obtained for these devices. In fact, as shown in Table 6, solar cells based on 1:3 and 1:4 ratio, display the highest FF of 0.56 and 0.57, respectively. On the other hand, the 1:2 based devices depicted a lower FF of 0.52, consistent with the lower charge carrier mobility obtained.
For all the devices, Jsc values are similar and this possibly can be attributed
to the not perfect energy alignment with PC71BM for achieving efficient
exciton splitting rather than to morphological issues as can be observed by investigations on the surface microstructure carried out through intermitted contact mode atomic force microscopy (AFM, Figure 21). A good intermixing between the donor and the acceptor materials is obtained and the topography and the phase images do not reveal obvious differences
between the three systems studied, supporting the hypothesis that the main limitations on of the system is due a to the low ELUMO offset rather than to
Figure 21. Topography(a,b,c) and phase (d,e,f) images of films TBDPTV:PC71BM 1:2,
1:3 and 1:4 respectively, on top of a layer of ZnO, as measured by intermittent contact mode atomic. Rms=2.29 nm.
External quantum efficiency (EQE) measurements have also been carried out for the best performing solar cell (Figure 22). An EQE signal around 950-1000 nm, even though very weak, is observed, suggesting an existing path towards charge generation from the polymer.
Figure 22. External quantum efficiency (EQE) curve of the TBDPTV:PC71BM (1:3)
As reported by Janssen et al.109, a fast recombination path becomes essential when the ELUMO of the acceptor become too shallow, leading to low Jsc
values. Noticeably, the rectification behavior of the device slightly improved with increasing the D:A ratio (Figure 22b). The Jsc calculated from the EQE
is 3.08 mA/cm-2, which is less than 10% smaller compared to the Jsc obtained
from the solar simulator.
In order to understand the transport properties of TBDPTV based solar cells, the charge carrier mobility μ of the aforementioned devices were determined by employing the technique of photoinduced charge carrier extraction by linearly increasing voltage (photo-CELIV)110. Charges are photogenerated by a strongly absorbed laser pulse and extracted after an adjustable delay
time. Figure 23 shows the photo-CELIV transients of the
TBDPTV:PC71BM system in the three different composition ratios (1:2, 1:3 and 1:4), which were recorded by applying a 2V/20 μs linearly increasing reverse bias pulse and a delay time (td) of 1 μs. From the measured photocurrent transients, the charge carrier mobility (μ) is calculated using the following equation:
where d is the active layer thickness, A is the voltage rise speed = U/dt, U is the applied voltage, tmax is the time corresponding to the maximum of
the extraction peak, and j(0) is the displacement current111.
The photocurrent transients in Figure 23 reveal that tmax occurs significantly
earlier for the 1:4 weight ratio. As a result, the calculated charge carrier mobility (μ) is higher for the 1:4 ratio (1.05±0.2)x10-5cm2V-1s-1, then for the
1:3 ratio (9.18±0.2)x10-6 cm2V-1s-1, and finally for the 1:2 ratio (7.50±0.1)x10-6 cm2V-1s-1, respectively.
Figure 23. Time-dependent photo-CELIV traces of TBDPTV-based solar cells at a fixed delay time of 1 μs.
3. BODIPY Small Molecules
Semiconducting organic small molecules have also attracted intense research attention and showed great promise in optoelectronic applications. The advantages of small molecules include well-defined molecular structures, high purity without batch-to batch variations, and the absence of end group contaminants. Moreover, crystalline small molecules exhibit high charge mobility due to their long-range order.
Organic semiconductors emitting in the NIR region are emerging as a promising class of materials with valuable optoelectronic properties. Among the appealing features there are solution processing, low-cost of fabrication, and the possibility of preparation on top of flexible, conformable or even stretchable substrates for organic electronic devices, such as organic (OLEDs) and polymer light-emitting diodes (PLEDs)115,116. In general, NIR emitters include organic semiconductors, metal-organic complexes, inorganic nanoparticles and hybrid organic-inorganic perovskite-like compounds117–120.
Although the quantum yield in this region of the spectrum is significantly lower than for materials emitting in the visible, owing to the so-called "energy-gap law", external quantum efficiencies (EQEs) spanning from ~ 9 % to ~ 24 % and have been achieved in OLEDs incorporating phosphorescent Pt-based porphyrins and carefully-designed derivatives121–
. While this is still significantly better than what is achievable with fluorescent NIR materials, the scope and applicability of phosphorescent OLEDs generates significant concerns both because of the use of heavy